PLEASE NOTE:
The new F3125 specification is a consolidation and replacement of six ASTM standards, including; A325, A325M, A490, A490M, F1852 (A325 TC), and F2280 (A490 TC). Until the F3125 specification is more widely used and until the A325 and A490 specifications have been eliminated by ASTM, we will continue to manufacture and sell A325 and A490 heavy hex structural bolts under their existing specification requirements, unless F3125 is referenced in the inquiry and/or purchase order.ASTM F3125 Grade F2280 (A490 TC)
Structural bolts, steel, heat treated, 120 ksi minimum tensile strength.
The ASTM F3125 Grade F2280, (Also known as A490 TC bolts) specification cover heat treated, steel, tension control bolt-nut-washer assemblies, also referred to as “sets.” These assemblies are capable of developing a minimum predetermined tension when installed by applying torque to the nut, while at the same time applying a counter torque to separate the spline end from the body of the bolt using an appropriate spline drive installation tool.
Formerly under the jurisdiction of Committee F16 on Fasteners, the F2280 specification was withdrawn in May 2016 and replaced by Specification F3125 for High Strength Structural Bolts, Steel and Alloy Steel, Heat Treated, 120 ksi Minimum Tensile Strength, Inch and Metric Dimensions.
Specifications
TYPES OF F3125 GRADE F2280 BOLTS | |
TYPE 1 | Alloy Steel with or without Boron (STANDARD) |
TYPE 3 | Weathering steel. |
M | Metric F1852. |
Bolt Diam. | E | F | H | T | S | |
Body Diam. | Head Diam. | Height | Thread Length | With Across Spline | ||
Max | Max | Max | Min | Basic | Basic | |
5/8-11 | 0.642 | 1.313 | 0.403 | 0.378 | 1.25 | 0.43 |
3/4-10 | 0.768 | 1.580 | 0.483 | 0.455 | 1.38 | 0.53 |
7/8-9 | 0.895 | 1.880 | 0.563 | 0.531 | 1.50 | 0.61 |
1-8 | 1.022 | 2.158 | 0.627 | 0.591 | 1.75 | 0.70 |
1 1/8-7 | 1.149 | 2.375 | 0.718 | 0.658 | 2.00 | 0.80 |
1 1/4-7 | 1.277 | 2.760 | 0.813 | 0.749 | 2.00 | 0.40 |
1 3/8-6 | 1.404 | 2.910 | 0.878 | 0.810 | 2.25 | 1.00 |
1 1/2-6 | 1.531 | 3.160 | 0.974 | 0.902 | 2.25 | 1.10 |
F3125 Grade F2280 Dimensions, Threads & Grade Marking | ||
Type 1 | Type 3 | |
Style Heavy Hex Bolts | ||
Dimensions, ASME^{B} | B18,2,6 | B18,2,6 |
Thread Fit, ASME^{B} | B1.1 UNC 2A | B1.1 UNC 2A |
Grade Marking^{A, D} | A490TC | A490TC |
^{B} Manufactured to the latest revision at the time of manufacture, UNC for inch series and Metric Coarse (MC) for Metric Series.
^{C} Previously used markings may be sold and used indefinitely, bolts must be manufactured to current marking requirements upon initial publication of this standard.
^{D} Other distinguishing markings for type 3 are permitted at the manufacturers option.
Source: The table above is inspired by Table 1 from the ASTM F3125 Standard that you can purchase on the ASTM Website
Chemical Requirements^{C} For ASTM F3125 Grade A490-1 & F2280-1 Bolts | |
Element | Alloy^{D} Steel with or Without Boron |
Carbon | 0.30 - 0.48^{A} |
Manganese, min | 0.60 min |
Phosphorus Max | 0.035 |
Sulfur Max | 0.040 |
Silicon | ^{B} |
Boron | 0.003 max |
Copper | ^{B} |
Nickel | ^{B} |
Chromium | ^{B} |
Vanadium | ^{B} |
Molybdenum | ^{B} |
Titanium | ^{B} |
^{B} Not Specified.
^{C} Product analysis that is outside the specified range is permitted provided it is within 10% of the value required of the heat analysis. For example Heat analysis C 0.30-0.52 = Product analysis C 0.27-0.57 or Phosphorus max Heat analysis 0.040 = Product analysis 0.044.
^{D} Steel, as defined by the American Iron and Steel Institute, shall be considered to be alloy when the maximum of the range given for the content of alloying elements exceeds one or more of the following limits: Manganese, 1.65 %; silicon, 0.60 %; copper, 0.60 % or in which a definite range or a definite minimum quantity of any of the following elements is specified or required within the limits of the recognized field of constructional alloy steels: aluminum, chromium up to 3.99 %, cobalt, columbium, molybdenum, nickel, titanium, tungsten, vanadium, zirconium, or any other alloying elements added to obtain a desired alloying effect.
Source: The table above is inspired by Table 2 from the ASTM F3125 Standard that you can purchase on the ASTM Website
Chemical Requirements^{C} For ASTM F3125 Grade A490-3 & F2280-3 Bolts | |
Element | Based on Corrosion Index^{E} |
Carbon | 0.30 - 0.53 max |
Manganese | 0.60 min |
Phosphorus Max | 0.035 |
Sulfur Max | 0.040 |
Silicon | ^{B} |
Boron | ^{B} |
Copper | 0.20 - 0.60^{E} |
Nickel | 0.20^{E,F} min |
Chromium | 0.45^{E} min |
Vanadium | ^{B} |
Molybdenum | 0.10^{E,F} min |
Titanium | ^{B} |
^{C} Product analysis that is outside the specified range is permitted provided it is within 10% of the value required of the heat analysis. For example Heat analysis C 0.30-0.52 = Product analysis C 0.27-0.57 or Phosphorus max Heat analysis 0.040 = Product analysis 0.044.
^{E} Type 3 bolts conforming to Table 2, or Type 3 bolts which have a copper minimum Heat Analysis of 0.20% and a Corrosion Index of 6 or higher as calculated from the Heat Analysis as described in Guide G101 Predictive method based on the data of Larabee and and Coburn shall be accepted: I = 26.01 (% Cu) + 3.88 (% Ni) + 1.20 (% Cr) + 1.49 (% Si) + 17.28 (% P) – 7.29 (% Cu) (% Ni) – 9.10 (%Ni) (% P) – 33.39 (% Cu)2
^{F} Either Nickel or Molybdenum must be present in the amount specified.
Source: The table above is inspired by Table 2 from the ASTM F3125 Standard that you can purchase on the ASTM Website
PERMITTED COATING^{H} | ||||
B695^{A} | F2329^{A} | F1136^{E,G} | F2833^{F,G} | |
Bolt | Mechanically Deposited Zinc | Hot-Dip Galvanized | Zinc/Aluminum | Zinc/Aluminum |
F2280 | Not Approved | Not Approved | Not Approved | Not Approved |
DIMENSIONAL LIMITS | BOLT PITCH DIAM. | BOLT PITCH DIAM. | BOLT PITCH DIAM. | BOLT PITCH DIAM. |
OS AFTER COATING^{C} | OS AFTER COATING^{C,D} | OS AFTER COATING^{C} | OS AFTER COATING^{C} | |
IN. | IN. | IN. | IN. | |
1/2-13 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
5/8-11 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
3/4-10 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
7/8-9 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
1-8 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
1 1/8-7 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
1 1/4-7 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
1 3/8-6 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
1 1/2-6 UNC | Not Approved | Not Approved | Not Approved | Not Approved |
^{C} Bolt pitch oversize limit in case of dispute. Material within the plain gauge limits which meets the coating thickness requirements and assembles freely need not be
measured to this tolerance.
^{D} Hot-Dip galvanized is typically tapped after coating. Others coatings are typically applied after nut tapping.
^{E} Grade 5 of this coating meets the supplementary lubrication requirements of A563 S1.
^{F} Grade 1 of this coating meets the supplementary lubrication requirements of A563 S1.
^{G} Nuts overtapped for coating for use with 150 ksi/1040 MPa minimum tensile strength fasteners shall be proof load tested to a minimum of 175,000 psi after overtapping.
^{H} Other metallic and non-metallic coatings may be used on 120 ksi/830 MPa minimum tensile fasteners upon agreement between the purchaser and user. Performance
requirements shall be specified by the purchaser and agreed to in writing. Coatings for 150 ksi/1040 MPa bolts must be qualified.
OS = over-size
Source: The table above is inspired by Table A1.1 from the ASTM F3125 Standard that you can purchase on the ASTM Website
F3125 Grade A490 & F2280 TENSILE STRENGHT REQUIREMENTS FOR BOLTS TESTED FULL SIZE | |||||
Stress Area^{A} | Tensile Min. | Tensile Max. | Proof Load^{C} Min. | Proof Load^{D} Min. | |
in. | in^{2}. | ft-lb | ft-lb | ft-lb | ft-lb |
1/2-13 | 0.142 in^{2}. | 21 300 ft-lb | 24 600 ft-lb | 17 050ft-lb | 18 500 ft-lb |
5/8-11 | 0.226 in^{2}. | 33 900 ft-lb | 39 100 ft-lb | 27 100 ft-lb | 29 400 ft-lb |
3/4-10 | 0.334 in^{2}. | 50 100 ft-lb | 57 800ft-lb | 40 100 ft-lb | 43 400 ft-lb |
7/8-9 | 0.462 in^{2}. | 69 300 ft-lb | 79 950 ft-lb | 55 450 ft-lb | 60 100 ft-lb |
1-8 | 0.606 in^{2}. | 90 900 ft-lb | 104 850 ft-lb | 72 700 ft-lb | 78 800 ft-lb |
1 1/8-7 | 0.763 in^{2}. | 114 450 ft-lb | 132 000 ft-lb | 91 550 ft-lb | 99 200 ft-lb |
1 1/4-7 | 0.969 in^{2}. | 145 350 ft-lb | 167 650 ft-lb | 116 300 ft-lb | 126 000 ft-lb |
1 3/8-6 | 1.155 in^{2}. | 173 250 ft-lb | 199 850 ft-lb | 138 600 ft-lb | 150 200 ft-lb |
1 1/2-6 | 1.405 in^{2}. | 210 750 ft-lb | 243 100 ft-lb | 168 600 ft-lb | 182 600 ft-lb |
Above Values Based On | * | 150 000 psi | 173 000 psi | 120 000 psi | 130 000 psi |
^{C} Proof load length measurement.
^{D} Alternative Proof load Yield Strength Method.
Source: The table above is inspired by Table 4 from the ASTM F3125 Standard that you can purchase on the ASTM Website
TENSILE STRENGHT REQUIREMENTS FOR SPECIMENS MACHINED BOLTS | |||||
F3125 Grade A490 & F2280 | Tensile, min. | Tensile, max. | Yeld min, | Elong. in 4D, min. % | Red. of Area min. % |
150 000 Psi | 173 000 psi | 130 000 Psi | 14 | 40 |
The table above is inspired by Table 5 from the ASTM F3125 Standard that you can purchase on the ASTM Website
CONNECTION TYPES | |
SC | Slip critical connection. |
N | Bearing type connection with threads included in the shear plane. |
X | Bearing-type connection with threads excluded from the shear plane. |
F3125 Grade A325, A490, F1852 & F2280 Matching Components | ||
Type 1 | Type 3 | |
Recommended Nut and Washer | ||
Plain Nut | A563 DH | A563 DH3 |
Suitable Alternative^{E} | DH3, D, C, C3 | C3 |
Coated Nut | A563 DH | A563 DH3 |
Flat, Bevel or Thick washer if used | F436-1 | F436-3 |
Source: The table above is inspired by Table 1 from the ASTM F3125 Standard that you can purchase on the ASTM Website
HARDNESS REQUIREMENTS FOR F3125 GRADE A490 & F2280 BOLTS | |||||
Brinell HB | Rockwell HRC | ||||
Min | Max | Min | Max | ||
Up to 1" INCLUSIVE | Less than 2D | 311 | 352 | 33 | 38 |
Up to 1" INCLUSIVE | 2D and longer | --- | 352 | --- | 38 |
Over 1" | Less than 3D | 311 | 352 | 33 | 38 |
Over 1" | 3D and longer | --- | 352 | --- | 38 |
10.2.1 Bolts shall conform to the hardness in Table 6. For
lots on which both hardness and tension tests are performed,
acceptance based on tensile requirements shall take precedence
in the event of low hardness readings.
Source: The table above is inspired by Table 6 from the ASTM F3125 Standard that you can purchase on the ASTM Website
Kegs & Skids Quantities
DIAM: 3/4 | FULL KEG | MINI KEG | ||||
LENGTH | BOLTS/KEG | LBS/KEG | BOLTS/MINI KEG | LBS/MINI KEG | BOLTS/SKID | LBS/SKID |
1 3/4 | N/A | N/A | 95 | 34.68 | 2565 | 936.23 |
2 | 280 | 190.40 | 90 | 61.20 | 2430 | 1698.30 |
2 1/4 | 270 | 191.70 | 85 | 60.35 | 2295 | 1629.45 |
2 1/2 | 250 | 185 | 80 | 59.20 | 2160 | 1598.40 |
2 3/4 | 250 | 192.50 | 80 | 61.60 | 2160 | 1663.20 |
3 | 220 | 176 | 75 | 60 | 2025 | 1620 |
3 1/4 | 210 | 174.30 | 75 | 62.25 | 2025 | 1680.75 |
3 1/2 | 200 | 172 | 70 | 60.20 | 1890 | 1625.40 |
3 3/4 | 190 | 169.10 | 70 | 62.30 | 1890 | 1682.10 |
4 | 170 | 156.40 | 70 | 64.40 | 1890 | 1738.8 |
4 1/4 | 170 | 161.50 | N/A | N/A | N/A | N/A |
4 1/2 | 170 | 166.60 | 70 | 68.60 | 1890 | 1852.20 |
4 3/4 | 160 | 163.20 | 70 | 71.40 | 1890 | 1927.80 |
5 | 150 | 157.50 | N/A | N/A | N/A | N/A |
5 1/2 | 140 | 155.40 | N/A | N/A | N/A | N/A |
6 | 130 | 152.10 | 50 | 58.50 | 1350 | 1579.50 |
Kegs and skids weight is an approximation. The real weight may slightly differ from what is shown here.
Other Lengths could be available upon request
DIAM: 7/8 | FULL KEG | MINI KEG | ||||
LENGTH | BOLTS/KEG | LBS/KEG | BOLTS/MINI KEG | LBS/MINI KEG | BOLTS/SKID | LBS/SKID |
2 | 200 | 208 | N/A | N/A | N/A | N/A |
2 1/4 | 190 | 207.10 | N/A | N/A | N/A | N/A |
2 1/2 | 180 | 204.30 | N/A | N/AE | N/A | N/A |
2 3/4 | 160 | 188 | N/A | N/A | N/A | N/A |
3 | 155 | 188.33 | N/A | N/A | N/A | N/A |
3 1/4 | 150 | 188.25 | N/A | N/A | N/A | N/A |
3 1/2 | 140 | 181.30 | N/A | N/A | N/A | N/A |
3 3/4 | 140 | 186.90 | N/A | N/A | N/A | N/A |
4 | 130 | 179.40 | N/A | N/A | N/A | N/A |
4 1/4 | 130 | 184.60 | N/A | N/A | N/A | N/A |
4 1/2 | 120 | 175.80 | N/A | N/A | N/A | N/A |
4 3/4 | 110 | 165.55 | N/A | N/A | N/A | N/A |
5 | 110 | 169.95 | N/A | N/A | N/A | N/A |
5 1/2 | 100 | 162.50 | N/A | N/A | N/A | N/A |
6 | 100 | 171.50 | N/A | N/A | N/A | N/A |
6 1/2 | 80 | 144.40 | N/A | N/A | N/A | N/A |
7 | 70 | 132.65 | N/A | N/A | N/A | N/A |
7 1/2 | 60 | 119.10 | N/A | N/A | N/A | N/A |
8 | N/A | N/A | N/A | N/A | N/A | N/A |
Kegs and skids weight is an approximation. The real weight may slightly differ from what is shown here.
Other Lengths could be available upon request
DIAM: 1'' | FULL KEG | MINI KEG | ||||
LENGTH | BOLTS/KEG | LBS/KEG | BOLTS/MINI KEG | LBS/MINI KEG | BOLTS/SKID | LBS/SKID |
2 1/4 | 130 | 178.10 | N/A | N/A | N/A | N/A |
2 1/2 | 120 | 171.60 | N/A | N/A | N/A | N/A |
2 3/4 | 120 | 178.20 | N/A | N/A | N/A | N/A |
3 | 110 | 169.40 | N/A | N/A | N/A | N/A |
3 1/4 | 110 | 176 | N/A | N/A | N/A | N/A |
3 1/2 | 100 | 165 | N/A | N/A | N/A | N/A |
3 3/4 | 100 | 171 | N/A | N/A | N/A | N/A |
4 | 90 | 158.40 | N/A | N/A | N/A | N/A |
4 1/4 | 90 | 163.80 | N/A | N/A | N/A | N/A |
4 1/2 | 80 | 150.40 | N/A | N/A | N/A | N/A |
4 3/4 | 80 | 155.20 | N/A | N/A | N/A | N/A |
5 | 80 | 158.40 | N/A | N/A | N/A | N/A |
5 1/2 | 70 | 146.30 | N/A | N/A | N/A | N/A |
6 | 60 | 132.60 | N/A | N/A | N/A | N/A |
6 1/2 | 50 | 116.50 | N/A | N/A | N/A | N/A |
7 | 40 | 98 | N/A | N/A | N/A | N/A |
7 1/2 | 30 | 77.10 | N/A | N/A | N/A | N/A |
8 | N/A | N/A | N/A | N/A | N/A | N/A |
Kegs and skids weight is an approximation. The real weight may slightly differ from what is shown here.
Other Lengths could be available upon request
DIAM: 1 1/8'' | FULL KEG* | MINI KEG | PER SKID INFOS | |||
LENGTH | BOLTS/KEG | LBS/KEG | BOLTS/MINI KEG | LBS/MINI KEG | BOLTS/SKID | LBS/SKID |
2 3/4 | 80 | 97.60 | N/A | N/A | N/A | N/A |
3 | 80 | 102.40 | N/A | N/A | N/A | N/A |
3 1/4 | 70 | 93.80 | N/A | N/A | N/A | N/A |
3 1/2 | 70 | 98.70 | N/A | N/A | N/A | N/A |
3 3/4 | 70 | 103.60 | N/A | N/A | N/A | N/A |
4 | 70 | 108.50 | N/A | N/A | N/A | N/A |
4 1/4 | 60 | 97.20 | N/A | N/A | N/A | N/A |
4 1/2 | 60 | 100.80 | N/A | N/A | N/A | N/A |
4 3/4 | 50 | 87.50 | N/A | N/A | N/A | N/A |
5 | 50 | 91 | N/A | N/A | N/A | N/A |
5 1/2 | 50 | 98 | N/A | N/A | N/A | N/A |
6 | 50 | 104.50 | N/A | N/A | N/A | N/A |
6 1/2 | 50 | 111 | N/A | N/A | N/A | N/A |
7 | 40 | 94 | N/A | N/A | N/A | N/A |
7 1/2 | 40 | 99.20 | N/A | N/A | N/A | N/A |
8 | 40 | 104.40 | N/A | N/A | N/A | N/A |
Kegs and skids weight is an approximation. The real weight may slightly differ from what is shown here.
Other Lengths could be available upon request